 
data_1 
 
_audit_creation_method            SHELXL-97 
_chemical_name_systematic 
; 
 ? 
; 
_chemical_name_common             ? 
_chemical_melting_point           ? 
_chemical_formula_moiety          'H4 K Na O11 V4'
_chemical_formula_sum 
 'H4 K Na O11 V4' 
_chemical_formula_weight          445.88 
 
loop_ 
 _atom_type_symbol 
 _atom_type_description 
 _atom_type_scat_dispersion_real 
 _atom_type_scat_dispersion_imag 
 _atom_type_scat_source 
 'O'  'O'   0.0106   0.0060 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
 'Na'  'Na'   0.0362   0.0249 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
 'H'  'H'   0.0000   0.0000 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
 'K'  'K'   0.2009   0.2494 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
 'V'  'V'   0.3005   0.5294 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
 
_symmetry_cell_setting            'monoclinic' 
_symmetry_space_group_name_H-M      'C2/c'
 
loop_ 
 _symmetry_equiv_pos_as_xyz 
 'x, y, z' 
 '-x, y, -z+1/2' 
 'x+1/2, y+1/2, z' 
 '-x+1/2, y+1/2, -z+1/2' 
 '-x, -y, -z' 
 'x, -y, z-1/2' 
 '-x+1/2, -y+1/2, -z' 
 'x+1/2, -y+1/2, z-1/2' 
 
_cell_length_a                    8.257(8) 
_cell_length_b                    15.475(16) 
_cell_length_c                    8.373(8) 
_cell_angle_alpha                 90.00 
_cell_angle_beta                  90.455(17) 
_cell_angle_gamma                 90.00 
_cell_volume                      1069.8(18) 
_cell_formula_units_Z             4 
_cell_measurement_temperature     293(2) 
_cell_measurement_reflns_used     1269 
_cell_measurement_theta_min       2.6325 
_cell_measurement_theta_max       27.5516
 
_exptl_crystal_description        'Prism' 
_exptl_crystal_colour             'Gray' 
_exptl_crystal_size_max           0.2000 
_exptl_crystal_size_mid           0.1500 
_exptl_crystal_size_min           0.0500 
_exptl_crystal_density_meas       ? 
_exptl_crystal_density_diffrn     2.768 
_exptl_crystal_density_method     'not measured' 
_exptl_crystal_F_000              856 
_exptl_absorpt_coefficient_mu     3.861 
_exptl_absorpt_correction_type    Multi-scan 
_exptl_absorpt_correction_T_min   0.8390 
_exptl_absorpt_correction_T_max   1.0000 
_exptl_absorpt_process_details    ? 
 
_exptl_special_details 
; 
 ? 
; 
 
_diffrn_ambient_temperature       293(2) 
_diffrn_radiation_wavelength      0.71073 
_diffrn_radiation_type            MoK\a 
_diffrn_radiation_source          'fine-focus sealed tube' 
_diffrn_radiation_monochromator   graphite 
_diffrn_measurement_device_type    'Mercury2(2*2 bin device) '
_diffrn_measurement_method        'CCD_Profile_fitting' 
_diffrn_detector_area_resol_mean   14.6306 
_diffrn_standards_number          ? 
_diffrn_standards_interval_count  ? 
_diffrn_standards_interval_time   ? 
_diffrn_standards_decay_%         ? 
_diffrn_reflns_number             5977 
_diffrn_reflns_av_R_equivalents   0.0427 
_diffrn_reflns_av_sigmaI/netI     0.0313 
_diffrn_reflns_limit_h_min        -10 
_diffrn_reflns_limit_h_max        10 
_diffrn_reflns_limit_k_min        -20 
_diffrn_reflns_limit_k_max        19 
_diffrn_reflns_limit_l_min        -10 
_diffrn_reflns_limit_l_max        10 
_diffrn_reflns_theta_min          2.63 
_diffrn_reflns_theta_max          27.37 
_reflns_number_total              1224 
_reflns_number_gt                 1103 
_reflns_threshold_expression      >2sigma(I) 
 
_computing_data_collection        'CrystalClear (Rigaku Inc., 2008)' 
_computing_cell_refinement        'CrystalClear (Rigaku Inc., 2008)' 
_computing_data_reduction         'CrystalClear (Rigaku Inc., 2008)' 
_computing_structure_solution     'SHELXS-97 (Sheldrick, 1990)' 
_computing_structure_refinement   'SHELXL-97 (Sheldrick, 1997)' 
_computing_molecular_graphics     ? 
_computing_publication_material   ? 
 
_refine_special_details 
; 
 Refinement of F² against ALL reflections.  The weighted R-factor wR and 
 goodness of fit S are based on F², conventional R-factors R are based 
 on F, with F set to zero for negative F². The threshold expression of 
 F² > 2sigma(F²) is used only for calculating R-factors(gt) etc. and is 
 not relevant to the choice of reflections for refinement.  R-factors based 
 on F² are statistically about twice as large as those based on F, and R- 
 factors based on ALL data will be even larger. 
; 
 
_refine_ls_structure_factor_coef  Fsqd  
_refine_ls_matrix_type            full 
_refine_ls_weighting_scheme       calc  
_refine_ls_weighting_details 
 'calc w=1/[σ²(Fo²)+(0.0384P)²+7.2228P] where P=(Fo²+2Fc²)/3' 
_atom_sites_solution_primary      direct 
_atom_sites_solution_secondary    difmap 
_atom_sites_solution_hydrogens    geom 
_refine_ls_hydrogen_treatment     mixed 
_refine_ls_extinction_method      none 
_refine_ls_extinction_coef        ? 
_refine_ls_number_reflns          1224 
_refine_ls_number_parameters      79 
_refine_ls_number_restraints      0 
_refine_ls_R_factor_all           0.0497 
_refine_ls_R_factor_gt            0.0438 
_refine_ls_wR_factor_ref          0.1006 
_refine_ls_wR_factor_gt           0.0967 
_refine_ls_goodness_of_fit_ref    1.131 
_refine_ls_restrained_S_all       1.131 
_refine_ls_shift/su_max           0.000 
_refine_ls_shift/su_mean          0.000 
 
loop_ 
 _atom_site_label 
 _atom_site_type_symbol 
 _atom_site_fract_x 
 _atom_site_fract_y 
 _atom_site_fract_z 
 _atom_site_U_iso_or_equiv 
 _atom_site_adp_type 
 _atom_site_occupancy 
 _atom_site_symmetry_multiplicity 
 _atom_site_calc_flag 
 _atom_site_refinement_flags 
 _atom_site_disorder_assembly 
 _atom_site_disorder_group 
V1 V 0.20676(7) 0.21022(4) 0.84364(7) 0.0100(2) Uani 1 1 d . . . 
V2 V 0.09725(7) 0.29539(4) 0.53839(7) 0.0101(2) Uani 1 1 d . . . 
Na Na 0.5000 0.65237(16) 0.2500 0.0222(5) Uani 1 2 d S . . 
K K 0.0000 0.48708(9) 0.2500 0.0263(3) Uani 1 2 d S . . 
O1 O 0.3947(3) 0.25148(19) 0.9608(3) 0.0126(6) Uani 1 1 d . . . 
O2 O 0.2913(3) 0.25407(19) 0.6450(3) 0.0122(6) Uani 1 1 d . . . 
O3 O 0.0000 0.2584(3) 0.7500 0.0127(8) Uani 1 2 d S . . 
O4 O 0.2084(4) 0.1064(2) 0.8345(3) 0.0203(7) Uani 1 1 d . . . 
O5 O 0.0960(4) 0.3992(2) 0.5230(3) 0.0215(7) Uani 1 1 d . . . 
O6 O 0.3358(5) 0.5438(2) 0.3526(4) 0.0456(11) Uani 1 1 d . . . 
H6A H 0.3753 0.4939 0.3278 0.055 Uiso 1 1 d R . . 
H6B H 0.3089 0.5405 0.4534 0.055 Uiso 1 1 d R . . 
 
 
_geom_special_details 
; 
 All esds (except the esd in the dihedral angle between two l.s. planes) 
 are estimated using the full covariance matrix.  The cell esds are taken 
 into account individually in the estimation of esds in distances, angles 
 and torsion angles; correlations between esds in cell parameters are only 
 used when they are defined by crystal symmetry.  An approximate (isotropic) 
 treatment of cell esds is used for estimating esds involving l.s. planes. 
; 
 
loop_ 
 _geom_bond_atom_site_label_1 
 _geom_bond_atom_site_label_2 
 _geom_bond_distance 
 _geom_bond_site_symmetry_2 
 _geom_bond_publ_flag 
V1 O4 1.609(3) . ? 
V1 O2 1.932(3) . ? 
V1 O1 1.937(3) . ? 
V1 O1 1.938(3) 7_557 ? 
V1 O3 2.016(2) . ? 
V1 V1 2.975(3) 7_557 ? 
V1 V2 3.009(2) . ? 
V1 V2 3.009(2) 2_556 ? 
V1 Na 3.321(3) 5_666 ? 
V1 K 3.979(3) 7_556 ? 
V2 O5 1.611(3) . ? 
V2 O1 1.931(3) 8_455 ? 
V2 O2 1.936(3) . ? 
V2 O2 1.953(3) 7_556 ? 
V2 O3 2.033(2) . ? 
V2 V2 2.962(3) 7_556 ? 
V2 V1 3.009(2) 2_556 ? 
V2 Na 3.368(3) 3_445 ? 
V2 K 3.891(3) 5_566 ? 
V2 K 3.904(3) . ? 
Na O6 2.327(4) . ? 
Na O6 2.327(4) 2_655 ? 
Na O2 2.412(3) 5_666 ? 
Na O2 2.412(3) 6_565 ? 
Na O1 2.471(3) 6_565 ? 
Na O1 2.471(3) 5_666 ? 
Na V1 3.321(3) 5_666 ? 
Na V1 3.321(3) 6_565 ? 
Na V2 3.368(3) 3 ? 
Na V2 3.368(3) 4 ? 
K O5 2.714(4) 5_566 ? 
K O5 2.714(4) 6_565 ? 
K O5 2.771(4) 2 ? 
K O5 2.771(4) . ? 
K O4 2.901(4) 8_455 ? 
K O4 2.901(4) 7_556 ? 
K O6 3.026(5) . ? 
K O6 3.026(5) 2 ? 
K V2 3.891(3) 5_566 ? 
K V2 3.891(3) 6_565 ? 
K V2 3.904(3) 2 ? 
O1 V2 1.931(3) 8_556 ? 
O1 V1 1.938(3) 7_557 ? 
O1 Na 2.471(3) 5_666 ? 
O2 V2 1.953(3) 7_556 ? 
O2 Na 2.412(3) 5_666 ? 
O3 V1 2.016(2) 2_556 ? 
O3 V2 2.033(2) 2_556 ? 
O4 K 2.901(4) 7_556 ? 
O5 K 2.714(4) 5_566 ? 
 
loop_ 
 _geom_angle_atom_site_label_1 
 _geom_angle_atom_site_label_2 
 _geom_angle_atom_site_label_3 
 _geom_angle 
 _geom_angle_site_symmetry_1 
 _geom_angle_site_symmetry_3 
 _geom_angle_publ_flag 
O4 V1 O2 107.87(14) . . ? 
O4 V1 O1 110.26(14) . . ? 
O2 V1 O1 91.53(12) . . ? 
O4 V1 O1 110.44(14) . 7_557 ? 
O2 V1 O1 141.40(15) . 7_557 ? 
O1 V1 O1 79.70(12) . 7_557 ? 
O4 V1 O3 110.99(15) . . ? 
O2 V1 O3 81.13(10) . . ? 
O1 V1 O3 138.38(16) . . ? 
O1 V1 O3 81.10(10) 7_557 . ? 
O4 V1 V1 116.93(11) . 7_557 ? 
O2 V1 V1 121.78(11) . 7_557 ? 
O1 V1 V1 39.87(7) . 7_557 ? 
O1 V1 V1 39.84(9) 7_557 7_557 ? 
O3 V1 V1 112.70(8) . 7_557 ? 
O4 V1 V2 113.57(11) . . ? 
O2 V1 V2 39.00(9) . . ? 
O1 V1 V2 121.32(9) . . ? 
O1 V1 V2 117.06(10) 7_557 . ? 
O3 V1 V2 42.24(4) . . ? 
V1 V1 V2 129.41(7) 7_557 . ? 
O4 V1 V2 117.41(11) . 2_556 ? 
O2 V1 V2 115.90(9) . 2_556 ? 
O1 V1 V2 110.88(10) . 2_556 ? 
O1 V1 V2 38.87(7) 7_557 2_556 ? 
O3 V1 V2 42.23(6) . 2_556 ? 
V1 V1 V2 74.03(5) 7_557 2_556 ? 
V2 V1 V2 80.86(5) . 2_556 ? 
O4 V1 Na 128.46(12) . 5_666 ? 
O2 V1 Na 45.80(8) . 5_666 ? 
O1 V1 Na 47.62(9) . 5_666 ? 
O1 V1 Na 108.94(10) 7_557 5_666 ? 
O3 V1 Na 106.75(12) . 5_666 ? 
V1 V1 Na 76.85(5) 7_557 5_666 ? 
V2 V1 Na 74.55(5) . 5_666 ? 
V2 V1 Na 114.13(8) 2_556 5_666 ? 
O4 V1 K 38.63(11) . 7_556 ? 
O2 V1 K 82.84(10) . 7_556 ? 
O1 V1 K 82.33(10) . 7_556 ? 
O1 V1 K 131.98(9) 7_557 7_556 ? 
O3 V1 K 136.21(9) . 7_556 ? 
V1 V1 K 110.41(5) 7_557 7_556 ? 
V2 V1 K 110.37(5) . 7_556 ? 
V2 V1 K 155.71(3) 2_556 7_556 ? 
Na V1 K 89.93(9) 5_666 7_556 ? 
O5 V2 O1 110.04(14) . 8_455 ? 
O5 V2 O2 111.76(14) . . ? 
O1 V2 O2 137.93(14) 8_455 . ? 
O5 V2 O2 109.30(14) . 7_556 ? 
O1 V2 O2 90.03(12) 8_455 7_556 ? 
O2 V2 O2 80.77(12) . 7_556 ? 
O5 V2 O3 110.37(15) . . ? 
O1 V2 O3 80.83(10) 8_455 . ? 
O2 V2 O3 80.57(10) . . ? 
O2 V2 O3 140.05(15) 7_556 . ? 
O5 V2 V2 117.40(11) . 7_556 ? 
O1 V2 V2 119.05(11) 8_455 7_556 ? 
O2 V2 V2 40.59(8) . 7_556 ? 
O2 V2 V2 40.18(8) 7_556 7_556 ? 
O3 V2 V2 113.47(9) . 7_556 ? 
O5 V2 V1 120.41(11) . . ? 
O1 V2 V1 112.03(9) 8_455 . ? 
O2 V2 V1 38.89(7) . . ? 
O2 V2 V1 110.85(10) 7_556 . ? 
O3 V2 V1 41.79(6) . . ? 
V2 V2 V1 74.09(5) 7_556 . ? 
O5 V2 V1 117.27(11) . 2_556 ? 
O1 V2 V1 39.05(8) 8_455 2_556 ? 
O2 V2 V1 113.16(10) . 2_556 ? 
O2 V2 V1 119.09(10) 7_556 2_556 ? 
O3 V2 V1 41.78(4) . 2_556 ? 
V2 V2 V1 125.28(7) 7_556 2_556 ? 
V1 V2 V1 77.00(5) . 2_556 ? 
O5 V2 Na 126.61(12) . 3_445 ? 
O1 V2 Na 46.44(8) 8_455 3_445 ? 
O2 V2 Na 107.77(10) . 3_445 ? 
O2 V2 Na 44.75(9) 7_556 3_445 ? 
O3 V2 Na 110.25(11) . 3_445 ? 
V2 V2 Na 74.42(5) 7_556 3_445 ? 
V1 V2 Na 112.93(8) . 3_445 ? 
V1 V2 Na 75.69(5) 2_556 3_445 ? 
O5 V2 K 34.19(11) . 5_566 ? 
O1 V2 K 107.28(10) 8_455 5_566 ? 
O2 V2 K 104.40(9) . 5_566 ? 
O2 V2 K 142.89(9) 7_556 5_566 ? 
O3 V2 K 76.26(12) . 5_566 ? 
V2 V2 K 133.49(4) 7_556 5_566 ? 
V1 V2 K 93.08(6) . 5_566 ? 
V1 V2 K 93.08(5) 2_556 5_566 ? 
Na V2 K 147.80(4) 3_445 5_566 ? 
O5 V2 K 36.11(11) . . ? 
O1 V2 K 84.48(10) 8_455 . ? 
O2 V2 K 134.53(9) . . ? 
O2 V2 K 84.69(11) 7_556 . ? 
O3 V2 K 132.24(10) . . ? 
V2 V2 K 113.41(5) 7_556 . ? 
V1 V2 K 156.52(3) . . ? 
V1 V2 K 111.58(5) 2_556 . ? 
Na V2 K 90.52(8) 3_445 . ? 
K V2 K 65.30(7) 5_566 . ? 
O6 Na O6 87.6(2) . 2_655 ? 
O6 Na O2 135.69(13) . 5_666 ? 
O6 Na O2 98.70(15) 2_655 5_666 ? 
O6 Na O2 98.70(15) . 6_565 ? 
O6 Na O2 135.69(13) 2_655 6_565 ? 
O2 Na O2 106.21(18) 5_666 6_565 ? 
O6 Na O1 87.81(13) . 6_565 ? 
O6 Na O1 155.14(12) 2_655 6_565 ? 
O2 Na O1 68.45(11) 5_666 6_565 ? 
O2 Na O1 69.17(11) 6_565 6_565 ? 
O6 Na O1 155.14(12) . 5_666 ? 
O6 Na O1 87.81(13) 2_655 5_666 ? 
O2 Na O1 69.17(11) 5_666 5_666 ? 
O2 Na O1 68.45(11) 6_565 5_666 ? 
O1 Na O1 105.97(17) 6_565 5_666 ? 
O6 Na V1 167.75(12) . 5_666 ? 
O6 Na V1 86.97(13) 2_655 5_666 ? 
O2 Na V1 35.05(7) 5_666 5_666 ? 
O2 Na V1 92.86(12) 6_565 5_666 ? 
O1 Na V1 92.55(11) 6_565 5_666 ? 
O1 Na V1 35.38(6) 5_666 5_666 ? 
O6 Na V1 86.97(13) . 6_565 ? 
O6 Na V1 167.75(12) 2_655 6_565 ? 
O2 Na V1 92.86(12) 5_666 6_565 ? 
O2 Na V1 35.05(7) 6_565 6_565 ? 
O1 Na V1 35.38(6) 6_565 6_565 ? 
O1 Na V1 92.55(11) 5_666 6_565 ? 
V1 Na V1 100.37(10) 5_666 6_565 ? 
O6 Na V2 110.25(11) . 3 ? 
O6 Na V2 127.06(12) 2_655 3 ? 
O2 Na V2 34.76(6) 5_666 3 ? 
O2 Na V2 91.86(11) 6_565 3 ? 
O1 Na V2 34.48(7) 6_565 3 ? 
O1 Na V2 91.90(12) 5_666 3 ? 
V1 Na V2 65.07(6) 5_666 3 ? 
V1 Na V2 65.17(6) 6_565 3 ? 
O6 Na V2 127.06(12) . 4 ? 
O6 Na V2 110.25(11) 2_655 4 ? 
O2 Na V2 91.86(11) 5_666 4 ? 
O2 Na V2 34.76(6) 6_565 4 ? 
O1 Na V2 91.90(12) 6_565 4 ? 
O1 Na V2 34.48(7) 5_666 4 ? 
V1 Na V2 65.17(6) 5_666 4 ? 
V1 Na V2 65.07(6) 6_565 4 ? 
V2 Na V2 97.84(10) 3 4 ? 
O5 K O5 99.11(15) 5_566 6_565 ? 
O5 K O5 144.41(12) 5_566 2 ? 
O5 K O5 79.86(12) 6_565 2 ? 
O5 K O5 79.86(12) 5_566 . ? 
O5 K O5 144.41(12) 6_565 . ? 
O5 K O5 121.17(15) 2 . ? 
O5 K O4 84.54(10) 5_566 8_455 ? 
O5 K O4 137.90(9) 6_565 8_455 ? 
O5 K O4 73.97(10) 2 8_455 ? 
O5 K O4 77.67(10) . 8_455 ? 
O5 K O4 137.90(9) 5_566 7_556 ? 
O5 K O4 84.54(10) 6_565 7_556 ? 
O5 K O4 77.67(10) 2 7_556 ? 
O5 K O4 73.97(10) . 7_556 ? 
O4 K O4 120.19(14) 8_455 7_556 ? 
O5 K O6 83.41(11) 5_566 . ? 
O5 K O6 74.84(11) 6_565 . ? 
O5 K O6 129.20(9) 2 . ? 
O5 K O6 69.68(10) . . ? 
O4 K O6 146.68(10) 8_455 . ? 
O4 K O6 56.88(11) 7_556 . ? 
O5 K O6 74.84(11) 5_566 2 ? 
O5 K O6 83.41(11) 6_565 2 ? 
O5 K O6 69.68(10) 2 2 ? 
O5 K O6 129.20(9) . 2 ? 
O4 K O6 56.88(11) 8_455 2 ? 
O4 K O6 146.68(10) 7_556 2 ? 
O6 K O6 146.28(17) . 2 ? 
O5 K V2 19.49(7) 5_566 5_566 ? 
O5 K V2 79.64(10) 6_565 5_566 ? 
O5 K V2 137.89(7) 2 5_566 ? 
O5 K V2 96.19(9) . 5_566 ? 
O4 K V2 98.37(8) 8_455 5_566 ? 
O4 K V2 135.82(7) 7_556 5_566 ? 
O6 K V2 79.15(9) . 5_566 ? 
O6 K V2 71.72(9) 2 5_566 ? 
O5 K V2 79.64(10) 5_566 6_565 ? 
O5 K V2 19.49(7) 6_565 6_565 ? 
O5 K V2 96.19(9) 2 6_565 ? 
O5 K V2 137.89(7) . 6_565 ? 
O4 K V2 135.82(7) 8_455 6_565 ? 
O4 K V2 98.37(8) 7_556 6_565 ? 
O6 K V2 71.72(9) . 6_565 ? 
O6 K V2 79.15(9) 2 6_565 ? 
V2 K V2 60.20(7) 5_566 6_565 ? 
O5 K V2 150.03(7) 5_566 2 ? 
O5 K V2 96.86(10) 6_565 2 ? 
O5 K V2 20.04(6) 2 2 ? 
O5 K V2 101.14(10) . 2 ? 
O4 K V2 66.74(7) 8_455 2 ? 
O4 K V2 68.73(8) 7_556 2 ? 
O6 K V2 125.40(8) . 2 ? 
O6 K V2 82.03(9) 2 2 ? 
V2 K V2 153.74(3) 5_566 2 ? 
V2 K V2 114.70(7) 6_565 2 ? 
O5 K V2 96.86(10) 5_566 . ? 
O5 K V2 150.03(7) 6_565 . ? 
O5 K V2 101.14(10) 2 . ? 
O5 K V2 20.04(6) . . ? 
O4 K V2 68.73(8) 8_455 . ? 
O4 K V2 66.74(7) 7_556 . ? 
O6 K V2 82.03(9) . . ? 
O6 K V2 125.40(8) 2 . ? 
V2 K V2 114.70(7) 5_566 . ? 
V2 K V2 153.74(3) 6_565 . ? 
V2 K V2 81.12(8) 2 . ? 
V2 O1 V1 137.28(17) 8_556 . ? 
V2 O1 V1 102.08(12) 8_556 7_557 ? 
V1 O1 V1 100.30(12) . 7_557 ? 
V2 O1 Na 99.08(11) 8_556 5_666 ? 
V1 O1 Na 97.00(11) . 5_666 ? 
V1 O1 Na 125.18(16) 7_557 5_666 ? 
V1 O2 V2 102.11(12) . . ? 
V1 O2 V2 135.64(17) . 7_556 ? 
V2 O2 V2 99.23(12) . 7_556 ? 
V1 O2 Na 99.14(11) . 5_666 ? 
V2 O2 Na 123.79(16) . 5_666 ? 
V2 O2 Na 100.48(12) 7_556 5_666 ? 
V1 O3 V1 136.6(2) 2_556 . ? 
V1 O3 V2 95.97(6) 2_556 2_556 ? 
V1 O3 V2 95.98(6) . 2_556 ? 
V1 O3 V2 95.98(6) 2_556 . ? 
V1 O3 V2 95.97(6) . . ? 
V2 O3 V2 147.3(2) 2_556 . ? 
V1 O4 K 121.12(15) . 7_556 ? 
V2 O5 K 126.32(16) . 5_566 ? 
V2 O5 K 123.85(15) . . ? 
K O5 K 100.14(12) 5_566 . ? 
Na O6 K 129.77(18) . . ? 
 
_diffrn_measured_fraction_theta_max    0.998 
_diffrn_reflns_theta_full              27.37 
_diffrn_measured_fraction_theta_full   0.998 
_refine_diff_density_max    1.741 
_refine_diff_density_min   -0.726 
_refine_diff_density_rms    0.148 
